Polymer Nanocomposite Dielectrics â€“ The Role of the nelsoj/ Polymer...
Embed Size (px)
Transcript of Polymer Nanocomposite Dielectrics â€“ The Role of the nelsoj/ Polymer...
Polymer Nanocomposite Dielectrics The Role of the Interface
M. Roy, J.K. Nelson, R.K. MacCrone, L.S. Schadler Rensselaer Polytechnic Institute
110 8th Street, Troy, NY 12180, USA
C.W. Reed 116 Woodhaven Dr.,
Scotia, NY 12302, USA
R. Keefe and W. Zenger Electric Power Research Institute
3412 Hillview Ave, Palo Alto, CA 94303, USA
The incorporation of silica nanoparticles into polyethylene increased the breakdown strength and voltage endurance significantly compared to the incorporation of micron scale fillers. In addition, dielectric spectroscopy showed a decrease in dielectric permittivity for the nanocomposite over the base polymer, and changes in the space charge distribution and dynamics have been documented. The most significant difference between micron scale and nanoscale fillers is the tremendous increase in interfacial area in nanocomposites. Because the interfacial region (interaction zone) is likely to be pivotal in controlling properties, the bonding between the silica and polyethylene was characterized using Fourier Transformed Infra-red (FTIR) spectroscopy, Electron Paramagnetic Resonance (EPR), and X-ray Photoelectron Spectroscopy (XPS) The picture which is emerging suggests that the enhanced interfacial zone, in addition to particle-polymer bonding, plays a very important role in determining the dielectric behavior of nanocomposites.
Index Terms Nanodielectrics, polyethylene, interface, dielectric strength, polymer nanocomposites, advanced materials, electrical insulation.
NANOPARTICLE-FILLED polymers provide advantages over micron-filled polymers because they provide resistance to degradation , and improvement in thermo-mechanical properties without causing a reduction in dielectric strength . For example, an increase in dielectric strength and a reduction in space charge has been documented for the case of nano-TiO2 filled epoxy resin over micron size TiO2 filled epoxy composites . Also, recently published results for electrical voltage endurance in these new materials indicate that very substantial (3 orders of magnitude) improvements in voltage endurance can be demonstrated. These improvements in dielectric properties observed for nano-filled polymers could be due to several factors: (i) the large surface area of Manuscript received on 7 March 2005, in final form on 31 May 2005.
nanoparticles which creates a large interaction zone or region of altered polymer behavior , (ii) changes in the polymer morphology due to the surfaces of particles , (iii) a reduction in the internal field caused by the decrease in size of the particles, (iv) changes in the space charge distribution [6, 7], and (v) a scattering mechanism. It should also be recognized that this technology also results in characteristic changes in non-electrical properties that have been found beneficial as detailed in references from a recent review paper .
The internal surfaces are critical in determining the properties of nano-filled materials. Nanoparticles have high surface area-to-volume ratio; particularly when the size decreases below 100 nm. This high surface area-to-
4000 3500 3000 2500 2000 1500 1000 500-1
Wave Number, [cm-1]
Dried vinylsilane-treated nanoparticles Vinylsilane-treated nanoparticles + XLPE
Figure 1. FTIR spectra. a, vinylsilane treated nano-silica powders; b, vinylsilane treated nanocomposite.
volume ratio means that for the same particle loading, nanocomposites will have a much greater interfacial area than microcomposites. This interfacial area leads to a significant volume fraction of polymer surrounding the particle that is affected by the particle surface and has properties different from the bulk polymer (interaction zone) . Since this interaction zone is much more extensive for nanocomposites than for microcomposites, it can have significant impact on properties [9, 10]. For example, depending upon the strength of the interaction between polymer and particle, this region can have a higher or lower mobility than the bulk material, and result in an increase  or decrease  in glass transition temperature . It has also been suggested that free volume in such interaction zones is altered by the introduction of nanofillers. Since, these interaction zones are likely to overlap at relatively low volume fractions in nanocomposites, a small amount of nanofiller has been found to impact the electrical behavior [12, 13]. Some authors have emphasized that the interaction zone around the particles is a quasi-conductive region which partially overlaps in the nanocomposites . These overlapped interface regions thus may allow charge dissipation, which, in turn, could be expected to improve the dielectric breakdown strength and voltage endurance characteristics.
Introduction of a second phase can also influence the breakdown strength of the dielectrics via a scattering mechanism  (i.e. an increase in path length of the carriers responsible for the breakdown processes) or, by changing the space charge distribution . It has been shown by some authors that when the size of the filler approaches the chain conformation length, they act cooperatively with the host structure either eliminating or suppressing Maxwell-Wagner polarization, which is well-known in the case of conventionally filled materials . Some recent results also suggest that it is the size of the filler that plays the most crucial role in terms of global properties (electrical, mechanical and thermal), rather than the chemistry of the particles . Finally, changes in morphology due to incorporating nanoparticles can influence the dielectric behavior of nanocomposites . The large surface area can also lead to changes in the morphology of semicrystalline polymers as observed by several groups [5, 17]. The breakdown strength of the intraspherulitic regions is higher than that of the interspherulitic regions and a change in the disorder within the spherulites or of the interspherulitic region can affect the breakdown strength.
The promise of unique electrical properties due to the mechanisms just described provides an incentive for investigating the dielectric properties of nano-filled materials. In order to obtain a better understanding of the role of the nanoparticles in the process of dielectric breakdown, lifetime, and space charge behavior, the interfacial region needs to be investigated. Interfacial characteristics are not only determined by the size-induced properties, but also the surface chemistry of the particles. Therefore, in this paper both as- received and
surface modified nanoscale silica was used since experience has indicated that chemical coupling can have beneficial effects . Therefore, in this paper both untreated and surface modified nanoscale silica was used, and the interface was characterized using several techniques. An attempt is made to connect the behavior at the interface to the breakdown strength, and provide some insight.
2 EXPERIMENTAL DETAILS 2.1 SYSTEM INVESTIGATED
The material studied here is a SiO2-polyethylene composite which has been formulated utilizing micro and nano particulates. The base polyethylene is a commercially available material already in use in the manufacturing of high-voltage (HV) extruded cross-linked underground cables. It is a high purity, filtered resin containing antioxidants. These additives are non-ionic and do not contribute to the base polymer conductivity. The polyethylene contains the cross-linking agent dicumyl peroxide (DCP), which reacts at temperatures above the compounding temperature creating a crosslinked matrix. Some untreated nanosilica was surface-modified with triethoxyvinylsilane.
Figure 1 shows FTIR spectra of vinylsilane-treated particles and vinylsilane-treated nanofillers in XLPE indicating that the surface treatment resulted in covalent bonding between the nanoparticles and the XLPE. There are two significant differences between these spectra: (1) many of the features of the particles (such as free silanol groups at 3747 cm-1 and a broad peak centered around 3500 cm-1) are gone, and (2) some new features are added. A peak at 1580-1680 cm-1 representing carbon-carbon double bond (-C=C-) which was present in the vinylsilane-treated particles (from the vinyl group) is replaced by the peak at 2860-2970 cm-1
Figure 2. Summary of the chemical-route for the attachment of the vinylsilane to the surface of the nanosilica particles, and the incorporation of the modified silica into XLPE.
Figure 3. SEM micrograph of XLPE with 5% untreated nanosilica
Table 1. Crystallinity and melting point data for XLPE materials from DSC measurements.
Sample Type Degree of crystallinity (%)
Melting Point (oC)
XLPE Only 45 1 103.2 1.4
5% untreated nanosilica + XLPE 44 1 109.0 0.5
5% vinylsilane treated nanosilica + XLPE 60 1 108.1 1.1
5% untreated microsilica + XLPE 44 1 108.3 1.2
representing the single bond of carbon (-CH2-CH2-) . This leads one to conclude that vinyltriethoxysilane is chemically bonded to silica particle on one end, and to polyethylene on the other. A schemati